DOI: 10.17188/1294237
title: Materials Data on Li3V3P8O29 by Materials Project

description: Li3V3P8O29 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are six inequivalent Li1+ sites. In the first Li1+ site, Li1+ is bonded to four O2- atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.94–2.20 Å. In the second Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.91–2.25 Å. In the third Li1+ site, Li1+ is bonded in a 4-coordinate geometry to four O2- atoms. There are a spread of Li–O bond distances ranging from 1.93–2.22 Å. In the fourth Li1+ site, Li1+ is bonded to four O2- atoms to form LiO4 tetrahedra that share corners with three VO6 octahedra and corners with four PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 68–70°. There are a spread of Li–O bond distances ranging from 1.87–2.30 Å. In the fifth Li1+ site, Li1+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Li–O bond distances ranging from 2.04–2.73 Å. In the sixth Li1+ site, Li1+ is bonded in a 6-coordinate geometry to six O2- atoms. There are a spread of Li–O bond distances ranging from 1.99–2.66 Å. There are six inequivalent V5+ sites. In the first V5+ site, V5+ is bonded to six O2- atoms to form VO6 octahedra that share a cornercorner with one LiO4 tetrahedra and corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.84–2.03 Å. In the second V5+ site, V5+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.85–1.94 Å. In the third V5+ site, V5+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.85–1.92 Å. In the fourth V5+ site, V5+ is bonded to six O2- atoms to form VO6 octahedra that share a cornercorner with one LiO4 tetrahedra and corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.82–2.00 Å. In the fifth V5+ site, V5+ is bonded to six O2- atoms to form VO6 octahedra that share a cornercorner with one LiO4 tetrahedra and corners with six PO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.85–2.01 Å. In the sixth V5+ site, V5+ is bonded to six O2- atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.84–2.00 Å. There are sixteen inequivalent P5+ sites. In the first P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedral tilt angles are 37°. There are a spread of P–O bond distances ranging from 1.47–1.61 Å. In the second P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 35–38°. There are a spread of P–O bond distances ranging from 1.47–1.60 Å. In the third P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 35–39°. There are a spread of P–O bond distances ranging from 1.48–1.60 Å. In the fourth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 25–30°. There are a spread of P–O bond distances ranging from 1.48–1.58 Å. In the fifth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and a cornercorner with one LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 30–35°. There are a spread of P–O bond distances ranging from 1.49–1.58 Å. In the sixth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 33–37°. There are a spread of P–O bond distances ranging from 1.47–1.61 Å. In the seventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–39°. There are a spread of P–O bond distances ranging from 1.49–1.61 Å. In the eighth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 35–37°. There are a spread of P–O bond distances ranging from 1.48–1.60 Å. In the ninth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–43°. There are a spread of P–O bond distances ranging from 1.47–1.61 Å. In the tenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedral tilt angles are 35°. There are a spread of P–O bond distances ranging from 1.48–1.60 Å. In the eleventh P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 43–44°. There are a spread of P–O bond distances ranging from 1.48–1.63 Å. In the twelfth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 26–28°. There are a spread of P–O bond distances ranging from 1.48–1.60 Å. In the thirteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and a cornercorner with one LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 29–31°. There are a spread of P–O bond distances ranging from 1.49–1.58 Å. In the fourteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–41°. There are a spread of P–O bond distances ranging from 1.48–1.61 Å. In the fifteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–45°. There are a spread of P–O bond distances ranging from 1.49–1.63 Å. In the sixteenth P5+ site, P5+ is bonded to four O2- atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 43–44°. There are a spread of P–O bond distances ranging from 1.47–1.63 Å. There are fifty-eight inequivalent O2- sites. In the first O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Li1+ and one P5+ atom. In the second O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the third O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one Li1+ and one P5+ atom. In the fourth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the fifth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the seventh O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the eighth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Li1+ and one P5+ atom. In the ninth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the tenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the eleventh O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the twelfth O2- site, O2- is bonded in a distorted trigonal non-coplanar geometry to one Li1+, one V5+, and one P5+ atom. In the thirteenth O2- site, O2- is bonded in a single-bond geometry to one P5+ atom. In the fourteenth O2- site, O2- is bonded in a single-bond geometry to one P5+ atom. In the fifteenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the sixteenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the seventeenth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one P5+ atom. In the eighteenth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the nineteenth O2- site, O2- is bonded in a distorted bent 150 degrees geometry to two P5+ atoms. In the twentieth O2- site, O2- is bonded in a 3-coordinate geometry to two Li1+ and one P5+ atom. In the twenty-first O2- site, O2- is bonded in a distorted bent 150 degrees geometry to one Li1+ and one P5+ atom. In the twenty-second O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the twenty-third O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one P5+ atom. In the twenty-fourth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the twenty-fifth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the twenty-sixth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the twenty-seventh O2- site, O2- is bonded in a distorted bent 150 degrees geometry to two P5+ atoms. In the twenty-eighth O2- site, O2- is bonded in a distorted bent 120 degrees geometry to one Li1+ and one P5+ atom. In the twenty-ninth O2- site, O2- is bonded in a 2-coordinate geometry to two Li1+ and one P5+ atom. In the thirtieth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the thirty-first O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the thirty-second O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the thirty-third O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the thirty-fourth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V5+, and one P5+ atom. In the thirty-fifth O2- site, O2- is bonded in a 2-coordinate geometry to two Li1+ and one P5+ atom. In the thirty-sixth O2- site, O2- is bonded in a 2-coordinate geometry to two Li1+ and one P5+ atom. In the thirty-seventh O2- site, O2- is bonded in a distorted bent 120 degrees geometry to two P5+ atoms. In the thirty-eighth O2- site, O2- is bonded in a distorted trigonal planar geometry to one Li1+, one V5+, and one P5+ atom. In the thirty-ninth O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the fortieth O2- site, O2- is bonded in a 3-coordinate geometry to one Li1+, one V5+, and one P5+ atom. In the forty-first O2- site, O2- is bonded in a bent 150 degrees geometry to one V5+ and one P5+ atom. In the forty-second O2- site, O2- is bonded in a linear geometry to one Li1+ and one P5+ atom. In the forty-third O2- site, O2- is bonded in a single-bond geometry t